received: 19 May 2016 accepted: 20 June 2016 Published: 07 July 2016
Fabrication of InGaN thin-film transistors using pulsed sputtering deposition Takeki Itoh1, Atsushi Kobayashi1, Kohei Ueno1, Jitsuo Ohta1,2 & Hiroshi Fujioka1,3 We report the first demonstration of operational InGaN-based thin-film transistors (TFTs) on glass substrates. The key to our success was coating the glass substrate with a thin amorphous layer of HfO2, which enabled a highly c-axis-oriented growth of InGaN films using pulsed sputtering deposition. The electrical characteristics of the thin films were controlled easily by varying their In content. The optimized InGaN-TFTs exhibited a high on/off ratio of ~108, a field-effect mobility of ~22 cm2 V−1 s−1, and a maximum current density of ~30 mA/mm. These results lay the foundation for developing highperformance electronic devices on glass substrates using group III nitride semiconductors. Thin-film transistors (TFTs) are key devices in large-area electronics and are fabricated on various types of amorphous substrates, such as glass or plastic1–3. Although hydrogenated amorphous silicon (a-Si:H)4 and amorphous oxide semiconductors such as InGaZnO (IGZO)5–7 are widely used as channel materials in TFTs, the electron mobility of these materials falls short of realizing high-performance electronic systems fabricated on amorphous materials. Conversely, group III nitride semiconductors, which have already been used as commercial transistors in ultrafast communication systems8,9, are promising materials for high-performance TFTs if they can be successfully accommodated on large-area amorphous substrates. In industrial applications, however, film growth of nitride semiconductors is usually achieved using metal-organic vapor-phase epitaxy10,11 at approximately 1000 °C12–14 in order to enhance the chemical reactivity of the raw materials. This temperature is obviously incompatible with large-area flat glass substrates. In order to overcome this problem and fabricate TFTs on conventional glass substrates, a novel growth technique that allows us to obtain high-quality nitride semiconductors on glass at low temperatures must be developed. Recently, the use of a new growth technique called pulsed sputtering deposition (PSD) was proposed for the preparation of group III nitrides15. During growth with PSD, high-energy film precursors formed in a plasma help produce high-quality group III nitride materials even at low temperatures (e.g., lower than 500 °C); this enables us to obtain InGaN films without phase separation and/or to employ thermally unstable substrates such as glass. In fact, we fabricated InGaN-based full-color light emitting diodes on graphene-covered amorphous SiO2 surfaces16. In this process, graphene was utilized as a buffer layer to promote c-axis orientation of the InGaN layers. Unfortunately, this orienting buffer layer is so conductive that it also acts as a leakage pathway when used as a substrate for TFTs. Therefore, fabrication of nitride-based TFTs on glass substrates requires an alternative orienting buffer layer of a highly insulating nature. In this study, we investigated the use of HfO2 as an orienting layer for InGaN film growth on glass substrates. We also explored the feasibility of producing InGaN-based TFTs on large-area amorphous substrates using a low-temperature PSD growth technique. Figure 1 shows XRD patterns of the InGaN films grown on glass substrates in this study. An InxGa1−xN film with x = 0.5, directly grown on a glass substrate, did not show any diffraction peaks because of poor crystallinity. Conversely, the InGaN films grown on HfO2-coated glass substrates exhibited peaks attributed to 0002 diffraction. The appearance of a sole 0002 diffraction peak in the XRD patterns indicates that highly c-axis-oriented InGaN films grow on HfO2-coated glass substrates. The full width at half maximum values of rocking curves for 0002 diffraction were larger than 1° for all samples. It was impossible to detect asymmetric diffraction of the InGaN films due to poor in-plane alignment. The In contents of the InGaN films prepared on the HfO2 buffer indicated in Fig. 1 are derived from the peak positions of the diffractions assuming that Vegard’s law is valid. Reflection high-energy electron diffraction observations (not shown) revealed that the InGaN films grown on HfO2-coated glass substrates are polycrystalline. An atomic force microscopic image of an In0.30Ga0.70N film 1 Institute of Industrial Science, The University of Tokyo, Tokyo 153-8505, Japan. 2PRESTO, Japan Science and Technology Agency, Saitama 332-0012, Japan. 3ACCEL, Japan Science and Technology Agency, Tokyo 102-0075, Japan. Correspondence and requests for materials should be addressed to H.F. (email: [email protected]
Scientific Reports | 6:29500 | DOI: 10.1038/srep29500
Figure 1. XRD 2θ scans of InxGa1−xN films with various In contents (x) grown on glass (upper) and a-HfO2-coated glass (lower). The In content indicated in the lower graph was calculated using Vegard’s law.
grown on a HfO2-coated glass substrate is shown in Fig. 2. Crystal grains with a size of ~10 nm are homogeneously grown on the substrate. The root-mean-square roughness of the InGaN surface was 1.8 nm, which is smooth enough to be used as a channel in a field-effect transistor. Coating glass substrates with HfO2 is also important for obtaining InGaN films with smooth surfaces and for suppressing electron scattering caused by rough interfaces between channel and gate dielectrics. Herein, 50 μm × 50 μm square mesas of 80-nm-thick c-axis-oriented InGaN were formed using an inductively coupled plasma (ICP) dry etching technique. Ti/Al electrodes were deposited on the corners of the InGaN mesas to perform van der Pauw Hall-effect measurements. The In content of the InGaN was evaluated with energy-dispersive X-ray spectroscopy (EDS). Figure 3 summarizes the relationship between the In composition, electron concentration, and electron mobility of the InGaN films. Note that since the Hall voltages for InGaN with In content x less than 0.6 were too low to be detected using our Hall-effect measurement setup, it was impossible to calculate the electron mobility and concentration of those InGaN. As the In composition decreases, the electron concentration of the InGaN monotonically decreases. An InGaN film with an In content of x = 0.60 has an electron concentration of ~1 × 1019 cm−3, whereas the electron concentration of a pure InN film is over 1 × 1020 cm−3. This result indicates that the electron concentration in InGaN films can be controlled by changing the In content. It is well known that as the In content in InGaN decreases, the Fermi-level stabilization energy drops from the conduction band into the forbidden gap17,18, which possibly explains the decrease in the electron concentration. Figure 3 also shows that the electron mobility of InGaN films decreases as the In content decreases. One of the reasons for this decrease is alloy scattering. Other possible explanations are the decrease in electron
Scientific Reports | 6:29500 | DOI: 10.1038/srep29500
Figure 2. Atomic force microscope image of an In0.30Ga0.70N film grown on an a-HfO2-coated glass substrate. The root-mean-square surface roughness was 1.8 nm, and the average grain size was ~10 nm.
Figure 3. Electron mobility and concentration of c-axis-oriented InxGa1−xN films on glass determined by Hall effect measurements. effective mass in InGaN with decreased In content and the formation of an energy barrier at the InGaN grain boundaries where the conduction band is possibly bent upward19. TFTs with InGaN channels were fabricated by photolithography and Cl2 ICP dry etching technologies. First, InGaN films were etched into 200 μm × 50 μm mesa structures. Source and drain electrodes (Ti/Al: 10 nm/30 nm) were subsequently deposited by sputtering, and a-HfO2 gate dielectrics were deposited on the InGaN films by atomic layer deposition (ALD) at 200 °C. Finally, gate electrodes (Au: 50 nm) were deposited by vacuum deposition. An optical microscope image and a schematic drawing of the transistor are shown in Fig. 4. Figure 5 shows the field-effect mobility of the InGaN TFTs. It is clear that the mobility strongly depends on the In content of the InGaN channel layer. As the In composition decreases, the mobility decreases from 4 to 0.16 cm2 V−1 s−1 (indicated as Region I), but rapidly increases to 22 cm2 V−1 s−1 at an In composition of 0.45 (Region II), before again decreasing to